UNIVERSITI TEKNIKAL MALAYSIA MELAKA (UTeM)
COMPLEX ADDITIVES INFLUENCE OF NiTe2
SYNTHESIZE BY ELECTRODEPOSITION
This report is submitted with requirement of the Universiti Teknikal Malaysia Melaka (UTeM) for the Bachelor Degree of Manufacturing Engineering (Engineering Materials)
AKHMAL HAKIM BIN HAKIMI
I hereby, declared this report entitled ‘Complex additives influence of NiTe2 thin film synthesize by electrodeposition’ is the results of my own research except as cited in
Signature : ………
Author’s Name : Akhmal Hakim Bin Hakimi
This report is submitted to the Faculty of Manufacturing Engineering of UTeM as a partial fulfillment to the requirements for the degree of Bachelor of Manufacturing Engineering (Engineering Materials) (Hons.). The member of the supervisory is as follow:
(Official Stamp of Principal Supervisor)
To my beloved parents and family members for their continuous support throughout my study.
To my supervisor and my co-supervisor for his advice and guidance in completing this research.
First of all, I would like to express my gratitude to Allah The Almighty for giving me the health to complete my Final Year Project succesfully. I would like to express my special thank for both my parents for their continuous support and help in order to complete my research. I would also like to express my deepest appreciatation and thank to my supervisor, Puan Siti Rahmah Binti Shamsuri and my co-supervisor, Professor Madya Dr. T. Joseph Sahaya Anand who willing to spare his time in guiding and share his experience for me to complete this research. Without his help, I would not be able to complete this research on time.
I would also like to thank all my friends who have support and willing to help me whenever I faced any problem in completing the research and the report.
TABLE OF CONTENT
Table of Content v
List of Tables viii
List of Figures ix
List of Abbreviations, Symbols and Nomenclatures x
CHAPTER 1: INTRODUCTION 1
1.1 Research Background 1
1.2 Problem Statement 2
1.3 Objectives 2
1.4 Scope 2
1.5 Outline of Project 2
CHAPTER 2: LITERATURE REVIEW 4
2.1 Introduction 4
2.3 Thin Film and Bulk Material 6
2.4 Thin Film Material 7
2.5 Factor that Affect Film Properties 8
2.6 Thin Film Coating 9
2.6.1 Physical Vapour Deposition (PVD) 10
2.6.2 Chemical Vapour Deposition (CVD) 10
188.8.131.52 Electrodeposition 11
2.7 Additive 14
2.7.1 Ethylenediaminetetraacetic acid (EDTA) 15
2.7.2 Triethanolamine (TEA) 17
2.8 Summary 19
CHAPTER 3: METHODOLOGY 20
3.1 Introduction 20
3.2 Sample Preparation 21
3.2.1 Preparation of ITO glass substrates 21
3.3. Cyclic Voltammetry and Electrodeposition Experiment 22
3.4 Thin Film Thickness Measurement 24
3.5 Structural Studies 24
vii CHAPTER 4: RESULTS AND DISCUSSION 28
4.1 Chapter Overview 28
4.2 Electrodeposition of NiTe2 thin film 28
4.3 Thin Film thickness measurement 30
4.4 Structural Studies 32
4.5 Surface Morphology and Compositional Studies by SEM and EDX 35
4.5.1. Surface Morphology by SEM 35
4.5.2 Compositional Study by EDX 37
4.6 Summary 40
CHAPTER 5: CONCLUSION AND RECOMMENDATION 41
5.1 Conclusion 41
5.2 Recommendation and Futher Studies 42
LIST OF TABLES
3.1 The electrolyte prepared for different condition 22 3.2 Technical specification of XRD machine utilized 25
4.1 Thin film thickness of deposited thin films 30
4.2 Comparison of JCPDS data and experimental ‘d’ value for TEA 33
LIST OF FIGURES
2.1 The evolution of the particle deposition growth and density of the particle 13
2.2 Images of the fast growth of the particle. 14
2.3 Titration curve of an EDTA complexometric titration 17 2.8 The chemical structure of triethanolamine (TEA) 18
3.1 Schematic setup for electrodeposition process 23
3.2 PW3040/60 X’PERT PRO X-ray diffraction system (PANalytical). 25
3.3 Scanning Electron Microscopy (SEM) 27
4.1 NiTe2 sample prepared with different molarity 29
4.2 Thin film thickness vs molarity 31
4.3 XRD pattern for different sample with present of TEA 33 4.4 XRD pattern for different sample with present of EDTA 34 4.5 Surface morphology of NiTe2 thin film deposited 36 4.6 Surface morphology of NiTe2 thin film deposited after annealing 36
process at 200°C
4.7 Surface morphology of NiTe2 thin film deposited after annealing 36 process at 300°C
4.8 Surface morphology of NiTe2 thin film deposited after annealing 37 process at 400°C
LIST OF ABBREVIATIONS, SYMBOLS AND
A - Ampere
Å - Angstrom
AACVD - Aerosol Assisted Chemical Vapour Deposition AFM - Atomic Force Microscopy
APCVD - Atmospheric Pressure Chemical Vapour Deposition Ag/AgCl - Argentums/ Argentums Chloride
Cd - Cadmium
CVD - Chemical Vapour Deposition
CV - Cyclic voltammetry
DLICVD - Direct Liquid Injection Chemical Vapour Deposition EDX - Energy disperse analysis X-Ray
EDTA - Ethylenediaminetetraacetic acid
FV - Frank-van der Merwe
Zn - Zinc
Hz - Hertz
ITO - Indium Tin Oxide
Kg/dm3 - Kilogram per cubic decimeter
Kpa - Kilo pascal
LPCVD - Low Pressure Chemical Vapour Deposition MgSe - Magnesium Selenide
Mo - Molybdenum
mm - Milimeters
Mpa - Mega pascal
MOCVD - Metal Organochemical Deposition
MPCVD - Microwave Plasma-assisted Chemical Vapour Deposition
Ni - Nickel
NiSe - Nickel selenide NiSO4 - Nickel Sulphate NiTe2 - Nickel Telluride PEC - Photoelectrochemical P/M - Powder Metallurgy
PECVD - Plasma Enhance Chemical Vapour Deposition PSA - Particle Size Analyzer
PVD - Physical Vapour Deposition
Se - Selenium
SEM - Scanning Electron Microscopy
Si - Silicon
SiC - Silicon Carbide
TEA - Triethanolamine
Te - Tellurium
TeO2 - Tellurium dioxide TFSC - Thin Film Solar Cell
TFPV - Thin Film Photovoltaic Cell TMC - Transition Metal Chalcogenides
UHVCVD - Ultra High Vacuum Chemical Vapour Deposition UTeM - Universiti Teknikal Malaysia Melaka
VW - Volmer-Weber
W - Tungsten
Wt - Weight percent
XRD - X-ray diffractometer
Zn - Zinc
% - Percent
°C - degree celcius
µm - Micrometre
1.1 Research Background
A thin-film solar cell (TFSC) is a solar cell that is made by depositing one or more thin layers (thin film) of photovoltaic material on a substrate. It also knows as a thin photovoltaic cell (TFPV). Recently, there has been a growing interest in multilayered semiconducting compounds basically consisting of transition metal dichalcogenides MX2 (M = Mo, W, Ni, Cd, Zn etc and X = S, Se, Te) (Anand, 2009). Thin film is the right and suitable material in the photovoltaic industry. Thin film is also suitable for the development of photoelectrochemical (PEC) and solar cell panels due to the semiconductor properties and also optical characteristic. A new thin film material such as transition metal chalcogenides NiX2 was introduced for solar energy to replace the conversional material.
2 1.2 Problem statement
This project is to study on the effect of additives for nickel telluride. Tellurium is difficult to deposit. The use of the additive is to improve adhesion of telluride and to produce the uniform coating. The other factor is the cost of its implementation for photovoltaic application. Solar panel including their component such as silicon is much more expensive compared to the other material.
a) To study the effect of additive influencing NiTe2 thin film by electrodeposition method along with deposition parameters.
b) To confirm the effectiveness of the additives in the thin film based on characterization technique using XRD and SEM/EDX.
c) To study the effect of annealing of NiTe2 thin film prepared by electrodeposition process.
The scope of this project lies on the effect of additives for nickel telluride thin film. Tellurium has the difficulty that is not easy to deposit. Other than that, experimental procedures and characterization technique also can be determined. The microstructural analysis is to be conducted by using scanning electron microscope (SEM), EDX and X-Ray Diffractometer that are capable to analyzing the sample.
1.5 Outline of Project
3 the research background, problem statement, objective, scope of study and the outline of the project.
Chapter two is a literature review presents the published literatures that are relevant to particular topic of this research, demonstrating the knowledge of any work before and the related theories and debates. In this chapter also provides the background of the new research, linking the new research to what preceded it.
In chapter 3, it will discuss the review of the methodology of the research. For example it explains more about the suitable method that are using for the experimental process. This chapter also include the review of the methodology carried out in order to produce the desired product or outcome of the project. The most appropriate method was chosen, allowing the sample to be further analyzed by suitable material characterization method.
In chapter 4 included the result and the conclusion for the experiment. The result can be determined after do the experiment.
This chapter describe substrate preparation of any thin film deposition technique or process and the best optimized parameters to synthesize the thin film. The step in thin film formation, the types of thin film coating methods and the complex additive that influence NiTe2 also will be discussed. Major factor controlling the deposition process were briefly described.
2.2 Thin Film
A thin-film solar cell (TFSC) is a cell that is made by depositing one or more thin layers (thin film) of photovoltaic material on a substrate. It also called a thin film photovoltaic cell (TFPV). A thin film is known as a low dimensional material synthesized by condensing, one by one, atomic, molecular, ionic species of matter. The electronic devices, optical coatings, instrument hard coatings and decorative parts in thin films have been used for more than a half century (Wasa et al., 2004).
5 Transition metal chalcogenides (TMCs) are semiconductors that can be used as an efficient photovoltaic material in the solar cells application. These chlcogenides have shown it potential on the solar cells application and actual application in thermoelectric, photoelectric devices, optoelectronics and also solar selective coatings (Ubale et al., 2013). The expected result has been obtained in the realization of photoelectrical solid state devices or solar cells by using TMC crystals. The thickness range of such a layer is wide and varies from a few nanometers to tens of micrometers. The thickness is typically less than several microns. Thin films are different from thick films. A thick film is defined as a low dimensional material created by thinning a three dimensional material or assembling large clusters, aggregats, and grains of atomic, molecular and ionic species (Wasa et al., 2004).
Transition metal nickel chalcogenides NiX2 (X – Se, S and Te) is a new thin film material for solar energy to replace the convensional material. Transition metal chalcogenide compound such as thin film can besuitablein the photovoltaic industry for the development of photoelectrochemical (PEC) and solar cell panels due to its characteristic by the semiconductors properties and also optical. This development has been proven by the high number of research publication on the application of TMC compounds in the PEC and solar cell industry (Mattox, 2010). The thin film development is more economical for the manufacturer because it reduces cost, energy required of the material and also their handling. A solid material is said to be in thin film form when it is grown as a thin layer on a solid substrate by controlled condensation of the individual atomic, molecular, or ionic species either by physical process or ultra chemical reactions. Basically, thin film deposition techniques are either purely physical such as evaporative method. The purely chemical method is such as gas and liquid phase chemical processes (Singh,n.d)
6 band gap with solar spectrum, high optical absorption band gap and good electrical conductivity. It also shows interesting electric and magnetic properties in this material. Polycrystalline electrodes are economically justified for solar cell applications where the large areas of substrates are necessary. Thus, the electrodeposition method is use to obtaining nickel telluride in the thin film form. The common preparation techniques that are used to deposition process are electrodeposition, chemical vapour deposition, spray pyrolysis, chemical bath deposition and sputtering (Hankare et al., 2010).
2.3 Thin Film and Bulk Material
Thin film is generally defined as a thin layer of material on a substrate. For without the substrate, a thin layer of the material would be called a foil (Christensen, 2000). Thin film is more different compared to bulk material due to its properties. Thin film not fully dense and it have different structures that have defect from bulk material and its properties are strongly influenced interface and surface effect (Christensen, 2000). These special properties of thin film make them difficult in electrical, magnetic, optical, thermal and mechanical properties than bulk material.
7 2.4 Thin Film Material
Thin films are deposited on a substrate by thermal evaporation, chemical decomposition, and the evaporation of source materials by their radiation of energetic species or photons. Thin-film growth exhibits the following features:
a) The birth of thin films of all materials created by any deposition technique starts with a random nucleation process followed by nucleation and growth stages.
b) Nucleation and growth stages are dependent upon various deposition conditions, such as growth temperature, growth rate and substrate chemistry. c) The nucleation stage can be modified significantly by external agencies such
as electron or ion bombardment.
d) Film microstructure, associated defect structure, and film stress depend on the deposition conditions at the nucleation stage.
e) The crystal phase and the orientation of the films are governed by the deposition conditions.
The features of thin film process have been shown to be the better material for solar cell applications and technologies as listed below.
a) The availability of variety of chemical, physical, electrochemical, plasma based and also hybrid deposition.
b) Microstructure of the thin film of most material can be varied from amorphous or noncrystalline to a highly oriented or epitaxial growth, depending on the technique, deposition parameter and substrate.
c) A wide selection of sizes, area, shapes and substrate are widely available. d) Relaxed solubility condition and phase diagram, allowing alloying and
doping process with well-matched materials.
e) Possible and practical to achieve easily different type of electronic function, single and tandem junction.
8 g) Bandgap, composition and other optoelectric properties can be graded in
desired manner in case of multi component materials.
h) Both surface and interface can be customized to provide surface electro field and interlayer diffusion barrier.
i) The desired optical reflectant or transmission characteristic, haze and optical trapping effects are achievable by modifying the surface
j) Intergration of unit process for manufacturing solar cell and intergration of individual solar cells can be easily accomplished.
k) Thin film process is classified as eco friendly, „green‟ process (Chopra et al., 2004).
2.5 Factor that Affect Film Properties
According to the Handbook of Physical Vapour Deposition (PVD) Processing by Donald M. Mattox, deposited thin films and coatings generally have unique properties compared to the material in bulk form. The four factors that affected the properties of a film of an exact material formed by an atomistic deposition process are:
a) Substrate the surface condition before and after cleaning and surface adjustment. For example surface morphology (roughness, inclusions, particulate contamination), surface chemistry (surface composition, contaminants), mechanical properties, surface flaws, outgassing, preferential nucleation sites, and the stability of the surface.
b) Details of the deposition process and system geometry. For example deposition process used angle-of-incidence distribution of the depositing adatom flux, substrate temperature, deposition rate, and gaseous contamination, concurrent energetic particle bombardment (flux, particle mass, and energy).